Pré-visualização3 páginas

by solving Eq. (10). The general solution gives .................(12) where r1 and r2 are the roots of Eq. (10)\u2019s character equa- tion and are expressed as where, FD\ufffd3pmur, Mp\ufffdpd 3r s/6, Fc\ufffdpd 3(r\ufffdr s)/6. Equation (12) shows that there is significant immigration of an inclusion toward the center of the swirling chamber, especially for inclusions of big size. In order to show the improved flow for inclusion aggre- gation, a contour plot of turbulent kinetic energy is given in Fig. 8. It shows that turbulent kinetic energy is confined in entry zone. Behind the dam and the weir, the flow of the swirling flow tundish is more stable than those of other kind of tundishes with different flow control device (Fig. 9). Consequently, more inclusions can float out and the metal/slag interface is calmer to prevent slag entrapment into steel. 6. Conclusions The flow patterns of a neotype tundish, swirling flow tundish with swirling chamber, have been studied by two types of turbulence models (standard and RNG k\u2013e turbu- lence models). The main conclusions derived from this study are as follows. (1) The numerical simulation results show that the RNG k\u2013e turbulence model is more suitable for this neo- type tundish and can get convergent results more easily than the standard k\u2013e turbulence model for strong curvature flows and flows with different Reynolds numbers in differ- ent areas. r F F M F M2 4 2\ufffd \ufffd \ufffd \ufffd( )/( )D D 2 p c p r F F M F M1 4 2\ufffd \ufffd \ufffd \ufffd( )/( )D D 2 p c p r R R r r r e r ert r t\ufffd \ufffd \ufffd \ufffd0 0 1 2 2 1 1 2( ) u r r a a r D D a r a D D a a r Dr \ufffd \ufffd \ufffd \ufffd \ufffd \ufffd \ufffd \ufffd \u3c9 \u3c9 2 1 4 2 4 2 2 ( ) ( ) / \uf8eb \uf8ed\uf8ec \uf8f6 \uf8f8\uf8f7 \uf8f1 \uf8f2\uf8f4 \uf8f3\uf8f4 du dt d r dt u dr dt r r\ufffd \ufffd 2 2 , \u3c0 \u3c1 \u3c0 \u3c1 \u3c1 \u3c9 \u3c0µ 6 6 33 3 2 0 0d du dt d R r d u ur r rs s\ufffd \ufffd \ufffd \ufffd \ufffd( ) ( ) ( ) ISIJ International, Vol. 45 (2005), No. 3 329 © 2005 ISIJ Fig. 7. Schematic of forces on inclusion particle and radial ve- locity distribution. Fig. 8. Predicted velocity contours on xy-plane at z/H\ufffd0.80. Fig. 9. Predicted velocity vectors at xy-plane. (a) z/H\ufffd0.95 (Ref. 22)), (b) section B at z/H\ufffd0.80. (2) The grid independent feature of this numerical model (RNG k\u2013e turbulence model) was verified by two kinds of grids with different node densities. (3) The unsymmetrical flow patterns of swirling flow tundish are mainly caused by the swirling flow out of the swirling chamber, partly because of turbulence fluctuation. (4) Under the centripetal force field, the inclusion can move to the center of swirling chamber and aggregate into a big one. The calm metal/slag interface and turbulent kinetic energy confinement in entry zone are favorable for inclu- sions to aggregation and floatation. Nomenclature: k : Turbulent kinetic energy kin : Turbulent kinetic energy at inlet ui : Mean velocity in the xi-direction uin : Mean velocity at inlet uq : Circumferential velocity in swirling chamber ur : Radial velocity in swirling chamber Frd : Drag force in radial direction Fad : Drag force in axial direction Ff : Floatation force on particle Fg : Gravity force on particle xi : Spatial coordinate in the i-direction p : Pressure Din : Diameters of inlet of long shroud D : Diameter of swirling chamber d : Diameter of inclusion particle H : Height of swirling chamber Fc : Centripetal force on particle a : Radius of central vortex Greek symbols e : Dissipation rate of kinetic energy e in : Dissipation rate of kinetic energy at inlet r : Density of fluid r s : Density of inclusion m : Molecular viscosity of Fluid m eff: Effective viscosity of fluid se, s k, C1, C2, Cm : Model constant for RNG and standard w : Rotational velocity REFERENCES 1) Y. He and Y. Sahai: Metall. Trans. B, 18B (1987), 81. 2) S. M. Lee, Y. S. Koo, T. Kang, I. R. Lee and Y. K. Shin: Proc. of The Sixth Int. Iron and Steel Cong., ISIJ, Tokyo, (1990). 3) P. K. Jha, S. K. Dash and S. Kumar: ISIJ Int., 41 (2001), 1437. 4) J. Palafox-Ramos, J. De J. Barreto, S. López-Ramírez and R. D. Morales: Ironmaking Steelmaking, 28 (2001), 101. 5) C. M. Fan, R. J. Shie and W. S. Hwang: Ironmaking Steelmaking, 30 (2003), 341. 6) P. K. Jha, R. Ranjan, S. S. Mondal and S. K. Dash: Int. J. Numerical Methods Heat Fluid Flow, 13 (2003), 964. 7) V. Yakhot and S. A. Orszag: J. Sci. Comput., 1 (1986), 3. 8) V. Yakhot and S. A. Orszag: Phys. Rev. Lett., 57 (1986), 1722. 9) G. Th. Analytis: Nucl. Eng. Des., 210 (2001), 177. 10) J. D. Ponser, C. R. Buchanan and D. Dunn-Rankin: Energy Buildings, 35 (2003), 515. 11) M. Yin, F. Shi and Z. Xu: Int. J. Eng. Sci., 34 (1996), 243. 12) F. Z. Sierra-Espinosa, C. J. Bates and T. O\u2019Doherty: Comput. Fluids, 29 (2000), 215. 13) B. W. Matthews, C. A. J. Fletcher and A. C. Patridge: Appl. Math. Model., 22 (1998), 965. 14) J. L. Xia, G. Yadigaroglu, Y. S. Liu, J. Chmidli and B. L. Smith: Int. J. Heat Mass Transfer, 41 (1998), 1485. 15) G. Mompean: Comput. Fluids, 27 (1998), 847. 16) D. Mazumdar, G. Yamanogl and R. I. L. Guthrie: Steel Res., 68 (1997), 293. 17) Y. Miki, S. Ogura and T. Fujii: Kawasaki Steel Giho, 35 (1996), 67. 18) Z. Zou, Q. Hou, S. Kuang and H. Li: Proc. 2nd Int. Conf. on Process Development in Iron and Steelmaking, Vol. 1, Metallurgical Research Institute AB, Luleå, (2004), 143. (9) B. E. Launder and D. B. Spalding: Comput. Methods Appl. Mech. Eng., 3 (1974), 269. 20) G. Solorio-Díaz, R. D. Morales, J. Palafax-Ramos, L. García- Demedices and A. Ramos-Bamderas: ISIJ Int., 44 (2004), 1024. 21) J. Wu, H. Ma and M. Zhou: Introduction to Vorticity and Vortex Dynamics, High Education Press, Beijing, (1993), 194. (in Chinese) 22) A. K. Sinha and Y. Sahai: ISIJ Int., 33 (1993), 556. ISIJ International, Vol. 45 (2005), No. 3 © 2005 ISIJ 330